Table 3. Condition of the Steels, As Received 



Alloy 



Condition 



Wrought Iron 



As fabricated pipe 



AISI CIOIO 



Hot rolled (mill) and pickled (laboratory) 



ASTM A36 



Hot rolled (mill) and pickled (laboratory) 



ASTM A387, D 



Hot rolled (mill) and pickled (laboratory) 



HSLA No. 1 



Water quenched from 1650° to 1750°F and 

 tempered at 1100° to 1275°F (mill), blast 

 cleaned (laboratory) 



HSLA No. 2 



Hot rolled and pickled 



HSLA No. 3 



Water quenched from 1650°F and tempered 

 at 1150° to 1200°F (mill), blast cleaned 

 (laboratory) 



HSLA No. 4 



Hot rolled (mill) and pickled (laboratory) 



HSLA No. 5 



o o 

 Water quenched from 1650 to 1750 F and 



tempered at 1150° to 1275°F (mill), blast 



cleaned (laboratory) 



HSLA No. 6 



Consumable electrode vacuum melt, hot 

 rolled, annealed, cleaned and oiled 



Ni-Co 



Consumable electrode vacuum melt, hot 

 rolled, annealed, cleaned and oiled 



AISI 4340 (200 KSI) 



Oil quenched from 1550°F, tempered for 1 

 hour at 750°F, blast cleaned (laboratory) 



AISI 4340 (150 KSI) 



Oil quenched from 1550°F, tempered for 1 

 hour at 1050 F, blast cleaned (laboratory) 



AISI Type 502 



Annealed and pickled. No. 1 sheet finish 

 (mill). 



continued 



20 



